மீக்கடத்திகளின் பட்டியல்
கீழே உள்ள அட்டவணை எளிய அமைப்பின் பொதுவான [[மீக்கடத்தி]]களின்  அளவுருக்கள் சிலவற்றைக் காட்டுகிறது. X:Y என்பது X என்ற பொருள் Y என்ற உறுப்பால் கலப்படம் செய்யப்பட்டுள்ளது என்பதை குறிப்பிடுகிறது. T என்பது பெருமப் பெயா்வு வெப்பநிலை [[கெல்வின்]] [K] அலகில் தரப்பட்டுள்ளது. H என்பது மாறுநிலை காந்தப்புலம் டெஸ்லா[T]  அலகில்.BCS என்பது மீக்கடத்துத்திறன் BCS கொள்கையில் விளக்கப்பட்டுள்ளதா இல்லையா எனக் குறிப்பிடுகிறது.
 {|class=&quot;wikitable sortable&quot;
 !வாய்ப்பாடு
 ! ''T''&lt;sub&gt;C&lt;/sub&gt; (K)
 ! ''H''&lt;sub&gt;C&lt;/sub&gt; (T)
 ! [[மீக்கடத்தி வகைபாடு|வகை]]
 ! [[BCS theory|BCS]]
 ! குறிப்புகள்
 |-
 |'''''தனிமம்'''''
 |
 |
 |
 |
 |
 |-
 |[[அலுமினியம்|Al]]
 |1.20
 |0.01
 |I
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1103/PhysRev.111.132| title = Superconducting Transition in Aluminum| journal = Physical Review| volume = 111| pages = 132| year = 1958| last1 = Cochran | first1 = J. F. | last2 = Mapother | first2 = D. E.| bibcode = 1958PhRv..111..132C}}&lt;/ref&gt;&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[காட்மியம்|Cd]]
 |0.52
 |0.0028
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e&gt;{{Cite journal | doi = 10.1103/RevModPhys.26.277| title = Superconducting Elements| journal = Reviews of Modern Physics| volume = 26| issue = 3| pages = 277| year = 1954| last1 = Eisenstein | first1 = J. | bibcode = 1954RvMP...26..277E}}&lt;/ref&gt;
 |-
 |[[Covalent superconductors#Diamond|Diamond:B]]
 |11.4
 |4
 |II
 |ஆம்
 |&lt;ref name=&quot;nature&quot;&gt;{{Cite journal | last1 = Ekimov | first1 = E. A. | last2 = Sidorov | first2 = V. A. | last3 = Bauer | first3 = E. D. | last4 = Mel'Nik | first4 = N. N. | last5 = Curro | first5 = N. J. | last6 = Thompson | first6 = J. D. | last7 = Stishov | first7 = S. M. | doi = 10.1038/nature02449 | title = Superconductivity in diamond | journal = Nature | volume = 428 | issue = 6982 | pages = 542–545 | year = 2004 | pmid =  15057827| pmc = }}&lt;/ref&gt;&lt;ref&gt;{{Cite journal | doi = 10.1088/1468-6996/9/4/044210| pmid = 27878027| title = Structure and superconductivity of isotope-enriched boron-doped diamond|pmc=5099641| journal = Science and Technology of Advanced Materials| volume = 9| issue = 4| pages = 044210| year = 2008| last1 = Ekimov | first1 = E. A. | last2 = Sidorov | first2 = V. A. | last3 = Zoteev | first3 = A. V. | last4 = Lebed | first4 = Y. B. | last5 = Thompson | first5 = J. D. | last6 = Stishov | first6 = S. M. | bibcode = 2008STAdM...9d4210E}} {{Open access}}&lt;/ref&gt;&lt;ref&gt;{{Cite journal | doi = 10.1016/j.diamond.2007.01.027| title = Superconducting properties of homoepitaxial CVD diamond| journal = Diamond and Related Materials| volume = 16| issue = 4–7| pages = 911| year = 2007| last1 = Takano | first1 = Y.| last2 = Takenouchi | first2 = T.| last3 = Ishii | first3 = S.| last4 = Ueda | first4 = S.| last5 = Okutsu | first5 = T.| last6 = Sakaguchi | first6 = I.| last7 = Umezawa | first7 = H.| last8 = Kawarada | first8 = H.| last9 = Tachiki | first9 = M.
 | bibcode = 2007DRM....16..911T}}&lt;/ref&gt;
 |-
 |[[காலியம்|Ga]]
 |1.083
 |0.0058
 |I
 |ஆம்
 |&lt;ref name=&quot;m&quot; /&gt;&lt;ref name=&quot;e&quot; /&gt;&lt;ref name=b1&gt;{{cite book|url=https://books.google.com/books?id=ULXZwEJeElYC&amp;pg=PA283|page=283|title=Atomic and electronic structure of solids|author=Kaxiras, Efthimios |publisher=Cambridge University Press|year=2003|isbn=0-521-52339-7}}&lt;/ref&gt;
 |-
 |[[ஆஃபினியம்|Hf]]
 |0.165
 |
 |I
 |ஆம்
 |&lt;ref name=m/&gt;
 |-
 |[[Mercury (element)|α-Hg]]
 |4.15
 |0.04
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Mercury (element)|β-Hg]]
 |3.95
 |0.04
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[இண்டியம்|In]]
 |3.4
 |0.03
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[இரிடியம்|Ir]]
 |0.14
 |0.0016&lt;ref name=b1/&gt;
 |I
 |ஆம்
 |&lt;ref name=m/&gt;
 |-
 |[[இலந்தனம்|α-La]]
 |4.9
 |
 |I
 |ஆம்
 |&lt;ref name=m&gt;{{Cite journal | doi = 10.1103/RevModPhys.35.1| title = Superconductivity| journal = Reviews of Modern Physics| volume = 35| pages = 1| year = 1963| last1 = Matthias | first1 = B. T.| last2 = Geballe | first2 = T. H.| last3 = Compton | first3 = V. B.| bibcode = 1963RvMP...35....1M}}&lt;/ref&gt;
 |-
 |[[இலந்தனம்|β-La]]
 |6.3
 |
 |I
 |ஆம்
 |&lt;ref name=m/&gt;
 |-
 |[[Molybdenum|Mo]]
 |0.92
 |0.0096
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=b1/&gt;
 |-
 |[[Niobium|Nb]]
 |9.26
 |0.82
 |II
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[ஓசுமியம்|Os]]
 |0.65
 |0.007
 |I
 |ஆம்
 |&lt;ref name=m/&gt;
 |-
 |[[Protactinium|Pa]]
 |1.4
 |
 |I
 |ஆம்
 |&lt;ref name=pa/&gt;
 |-
 |[[ஈயம்|Pb]]
 |7.19
 |0.08
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[இரேனியம்|Re]]
 |2.4
 |0.03
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;&lt;ref&gt;{{Cite journal | doi = 10.1103/PhysRev.88.309| title = Superconductivity of Rhenium| journal = Physical Review| volume = 88| issue = 2| pages = 309| year = 1952| last1 = Daunt | first1 = J. G.| last2 = Smith | first2 = T. S.| bibcode = 1952PhRv...88..309D}}&lt;/ref&gt;
 |-
 |[[Ruthenium|Ru]]
 |0.49
 |0.005
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Covalent superconductors#Silicon|Si:B]]
 |0.4
 |0.4
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1038/nature05340| pmid = 17122852| title = Superconductivity in doped cubic silicon| journal = Nature| volume = 444| issue = 7118| pages = 465| year = 2006| last1 = Bustarret | first1 = E.| last2 = Marcenat | first2 = C.| last3 = Achatz | first3 = P.| last4 = Kačmarčik | first4 = J.| last5 = Lévy | first5 = F.| last6 = Huxley | first6 = A.| last7 = Ortéga | first7 = L.| last8 = Bourgeois | first8 = E.| last9 = Blase | first9 = X.| last10 = Débarre | first10 = D.| last11 = Boulmer | first11 = J.| bibcode = 2006Natur.444..465B}}&lt;/ref&gt;
 |-
 |[[Tin|Sn]]
 |3.72
 |0.03
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Tantalum|Ta]]
 |4.48
 |0.09
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Technetium|Tc]]
 |7.46–11.2
 |0.04
 |II
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Thorium|α-Th]]
 |1.37
 |0.013
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Titanium|Ti]]
 |0.39
 |0.01
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Thallium|Tl]]
 |2.39
 |0.02
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Uranium|α-U]]
 |0.68
 |
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=pa/&gt;
 |-
 |[[Uranium|β-U]]
 |1.8
 |
 |I
 |ஆம்
 |&lt;ref name=pa/&gt;
 |-
 |[[Vanadium|V]]
 |5.03
 |1
 |II
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[Tungsten|α-W]]
 |0.015
 |0.00012
 |I
 |ஆம்
 |&lt;ref name=b1/&gt;&lt;ref name=pa&gt;{{Cite journal | doi = 10.1103/PhysRevLett.15.860| title = Superconductivity of Protactinium| journal = Physical Review Letters| volume = 15| issue = 22| pages = 860| year = 1965| last1 = Fowler | first1 = R. D.| last2 = Matthias | first2 = B. T.| last3 = Asprey | first3 = L. B.| last4 = Hill | first4 = H. H.| last5 = Lindsay | first5 = J. D. G.| last6 = Olsen | first6 = C. E.| last7 = White | first7 = R. W.| bibcode = 1965PhRvL..15..860F}}&lt;/ref&gt;&lt;ref name=al&gt;{{Cite journal | doi = 10.1109/TASC.2005.849033| title = Tuning of Tungsten Thin Film Superconducting Transition Temperature for Fabrication of Photon Number Resolving Detectors| journal = IEEE Transactions on Appiled Superconductivity| volume = 15| issue = 2| pages = 3528| year = 2005| last1 = Lita | first1 = A. E. | last2 = Rosenberg | first2 = D.| last3 = Nam | first3 = S.| last4 = Miller | first4 = A. J. | last5 = Balzar | first5 = D.| last6 = Kaatz | first6 = L. M. | last7 = Schwall | first7 = R. E. }}&lt;/ref&gt;
 |-
 |[[Tungsten|β-W]]
 |1–4
 |
 |
 |
 |&lt;ref name=al/&gt;
 |-
 |[[zinc|Zn]]
 |0.855
 |0.005
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |[[zirconium|Zr]]
 |0.55
 |0.014
 |I
 |ஆம்
 |&lt;ref name=m/&gt;&lt;ref name=e/&gt;
 |-
 |'''''சேர்மங்கள்'''''
 |
 |
 |
 |
 |
 |-
 |Ba&lt;sub&gt;8&lt;/sub&gt;Si&lt;sub&gt;46&lt;/sub&gt;
 |8.07
 |0.008
 |II
 |ஆம்
 |&lt;ref name=&quot;Rachi2006&quot;&gt;{{Cite journal |doi=10.1016/j.stam.2006.04.006 | title = Sp&lt;sup&gt;3&lt;/sup&gt;-network superconductors made from IVth-group elements| journal = Science and Technology of Advanced Materials| volume = 7| pages = S88| year = 2006| last1 = Rachi | first1 = T. | last2 = Kumashiro | first2 = R. | last3 = Fukuoka | first3 = H. | last4 = Yamanaka | first4 = S. | last5 = Tanigaki | first5 = K. | bibcode = 2006STAdM...7S..88R}} {{Open access}}&lt;/ref&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;6&lt;/sub&gt;Ca]]
 |11.5
 |0.95
 |II
 |
 |&lt;ref name=cac6&gt;{{Cite journal | doi = 10.1088/1468-6996/9/4/044102| pmid = 27878015| title = Synthesis and superconducting properties of CaC&lt;sub&gt;6&lt;/sub&gt;| journal = Science and Technology of Advanced Materials| volume = 9| issue = 4| pages = 044102| year = 2008| last1 = Emery | first1 = N. | last2 = Hérold | first2 = C. | last3 = Marêché | first3 = J. F. O. | last4 = Lagrange | first4 = P. | bibcode = 2008STAdM...9d4102E|pmc= 5099629}} {{Open access}}&lt;/ref&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;6&lt;/sub&gt;Li&lt;sub&gt;3&lt;/sub&gt;Ca&lt;sub&gt;2&lt;/sub&gt;]]
 |11.15
 |
 |II
 |
 |&lt;ref name=cac6/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;8&lt;/sub&gt;K]]
 |0.14
 |
 |II
 |
 |&lt;ref name=cac6/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;8&lt;/sub&gt;KHg]]
 |1.4
 |
 |II
 |
 |&lt;ref name=cac6/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;6&lt;/sub&gt;K]]
 |1.5
 |
 |II
 |
 |&lt;ref name=gic&gt;{{Cite journal | doi = 10.1016/0379-6779(89)90424-4| title = Superconductivity of GIC with Li, Na and K| journal = Synthetic Metals| volume = 34| pages = 455| year = 1989| last1 = Belash | first1 = I. T. | last2 = Zharikov | first2 = O. V. | last3 = Palnichenko | first3 = A. V. }}&lt;/ref&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;3&lt;/sub&gt;K]]
 |3.0
 |
 |II
 |
 |&lt;ref name=gic/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;3&lt;/sub&gt;Li]]
 |&lt;0.35
 |
 |II
 |
 |&lt;ref name=gic/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;2&lt;/sub&gt;Li]]
 |1.9
 |
 |II
 |
 |&lt;ref name=gic/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;3&lt;/sub&gt;Na]]
 |2.3–3.8
 |
 |II
 |
 |&lt;ref name=gic/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;2&lt;/sub&gt;Na]]
 |5.0
 |
 |II
 |
 |&lt;ref name=gic/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;8&lt;/sub&gt;Rb]]
 |0.025
 |
 |II
 |
 |&lt;ref name=cac6/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;6&lt;/sub&gt;Sr]]
 |1.65
 |
 |II
 |
 |&lt;ref name=cac6/&gt;
 |-
 |[[Covalent superconductors#Intercalated graphite|C&lt;sub&gt;6&lt;/sub&gt;Yb]]
 |6.5
 |
 |II
 |
 |&lt;ref name=cac6/&gt;
 |-
 |[[Fullerene#Superconductivity|C&lt;sub&gt;60&lt;/sub&gt;Cs&lt;sub&gt;2&lt;/sub&gt;Rb]]
 |33
 |
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1038/352222a0| title = Superconductivity at 33 K in Cs&lt;sub&gt;x&lt;/sub&gt;Rb&lt;sub&gt;y&lt;/sub&gt;C&lt;sub&gt;60&lt;/sub&gt;| journal = Nature| volume = 352| issue = 6332| pages = 222| year = 1991| last1 = Tanigaki | first1 = K.| last2 = Ebbesen | first2 = T. W.| last3 = Saito | first3 = S.| last4 = Mizuki | first4 = J.| last5 = Tsai | first5 = J. S.| last6 = Kubo | first6 = Y.| last7 = Kuroshima | first7 = S.| bibcode = 1991Natur.352..222T}}&lt;/ref&gt;
 |-
 |[[Fullerene#Superconductivity|C&lt;sub&gt;60&lt;/sub&gt;K&lt;sub&gt;3&lt;/sub&gt;]]
 |19.8
 |0.013
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1126/science.256.5060.1190| pmid = 17795215| title = Synthesis and Electronic Transport of Single Crystal K&lt;sub&gt;3&lt;/sub&gt;C&lt;sub&gt;60&lt;/sub&gt;| journal = Science| volume = 256| issue = 5060| pages = 1190| year = 1992| last1 = Xiang | first1 = X. -D.| last2 = Hou | first2 = J. G.| last3 = Briceno | first3 = G.| last4 = Vareka | first4 = W. A.| last5 = Mostovoy | first5 = R.| last6 = Zettl | first6 = A.| last7 = Crespi | first7 = V. H.| last8 = Cohen | first8 = M. L.| bibcode = 1992Sci...256.1190X}}&lt;/ref&gt;&lt;ref name=&quot;Rachi2006&quot; /&gt;
 |-
 |[[Fullerene#Superconductivity|C&lt;sub&gt;60&lt;/sub&gt;Rb&lt;sub&gt;X&lt;/sub&gt;]]
 |28
 |
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1103/PhysRevLett.66.2830| title = Superconductivity at 28 K in Rb&lt;sub&gt;x&lt;/sub&gt;C&lt;sub&gt;60&lt;/sub&gt;| journal = Physical Review Letters| volume = 66| issue = 21| pages = 2830–2832| year = 1991| last1 = Rosseinsky | first1 = M.| last2 = Ramirez | first2 = A.| last3 = Glarum | first3 = S.| last4 = Murphy | first4 = D.| last5 = Haddon | first5 = R.| last6 = Hebard | first6 = A.| last7 = Palstra | first7 = T.| last8 = Kortan | first8 = A.| last9 = Zahurak | first9 = S.| last10 = Makhija | first10 = A. | pmid=10043627}}&lt;/ref&gt;
 |-
 |FeB&lt;sub&gt;4&lt;/sub&gt;
 |2.9
 |
 |I
 |
 |&lt;ref&gt;{{cite web|url=http://www.kurzweilai.net/first-fully-computer-designed-superconductor |title=First fully computer-designed superconductor |publisher=KurzweilAI |accessdate=2013-10-11}}&lt;/ref&gt;
 |-
 |[[Indium(III) nitride|InN]]
 |3
 |
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1016/j.stam.2006.06.004 | title = Electronic structure of superconducting InN| journal = Science and Technology of Advanced Materials| volume = 7| pages = S112| year = 2006| last1 = Inushima | first1 = T. | bibcode = 2006STAdM...7S.112I}} {{Open access}}&lt;/ref&gt;
 |-
 |[[Indium(III) oxide|In&lt;sub&gt;2&lt;/sub&gt;O&lt;sub&gt;3&lt;/sub&gt;]]
 |3.3
 |~3
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1088/1468-6996/9/4/044208 | pmid = 27878025| title = Superconductivity in transparent zinc-doped In&lt;sub&gt;2&lt;/sub&gt;O&lt;sub&gt;3&lt;/sub&gt; films having low carrier density|pmc=5099639| journal = Science and Technology of Advanced Materials| volume = 9| issue = 4| pages = 044208| year = 2008| last1 = Makise | first1 = K. | last2 = Kokubo | first2 = N. | last3 = Takada | first3 = S. | last4 = Yamaguti | first4 = T. | last5 = Ogura | first5 = S. | last6 = Yamada | first6 = K. | last7 = Shinozaki | first7 = B. | last8 = Yano | first8 = K. | last9 = Inoue | first9 = K. | last10 = Nakamura | first10 = H. | bibcode = 2008STAdM...9d4208M}} {{Open access}}&lt;/ref&gt;
 |-
 |[[Lanthanum hexaboride|LaB&lt;sub&gt;6&lt;/sub&gt;]]
 |0.45
 |
 |
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1103/PhysRevB.25.1589| title = Electronic structure and superconductivity in metal hexaborides| journal = Physical Review B| volume = 25| issue = 3| pages = 1589| year = 1982| last1 = Schell | first1 = G.| last2 = Winter | first2 = H.| last3 = Rietschel | first3 = H.| last4 = Gompf | first4 = F.| bibcode = 1982PhRvB..25.1589S}}&lt;/ref&gt;
 |-
 |[[Magnesium diboride|MgB&lt;sub&gt;2&lt;/sub&gt;]]
 |39
 |74
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal|title=Superconductivity at 39 K in magnesium diboride | doi = 10.1038/35065039| pmid = 11242039|bibcode=2001Natur.410...63N|url=http://www.researchgate.net/publication/12090250_Superconductivity_at_39_K_in_magnesium_diboride| year = 2001| last1 = Nagamatsu | first1 = J. | journal = Nature| volume = 410| issue = 6824| pages = 63| last2 = Nakagawa | first2 = N. | last3 = Muranaka | first3 = T. | last4 = Zenitani | first4 = Y. | last5 = Akimitsu | first5 = J. }}&lt;/ref&gt;
 |-
 |Nb&lt;sub&gt;3&lt;/sub&gt;Al
 |18
 |
 |II
 |ஆம்
 |&lt;ref name=m/&gt;
 |-
 |[[Niobium-germanium|Nb&lt;sub&gt;3&lt;/sub&gt;Ge]]
 |23.2
 |37
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1007/BF00114941| title = Preparation of Nb&lt;sub&gt;3&lt;/sub&gt;Ge films by chemical transport reaction and their critical properties| journal = Journal of Low Temperature Physics| volume = 34| issue = 5–6| pages = 569| year = 1979| last1 = Oya | first1 = G. I. | last2 = Saur | first2 = E. J.| bibcode = 1979JLTP...34..569O}}&lt;/ref&gt;
 |-
 |[[Niobium monoxide|NbO]]
 |1.38
 |
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1007/BF00660068| title = Superconductivity in the TiO and NbO systems| journal = Journal of Low Temperature Physics| volume = 7| issue = 3–4| pages = 291| year = 1972| last1 = Hulm | first1 = J. K.| last2 = Jones | first2 = C. K.| last3 = Hein | first3 = R. A.| last4 = Gibson | first4 = J. W.| bibcode = 1972JLTP....7..291H}}&lt;/ref&gt;
 |-
 |[[Niobium nitride|NbN]]
 |16
 |
 |II
 |ஆம்
 |&lt;ref name=m/&gt;
 |-
 |[[Niobium-tin|Nb&lt;sub&gt;3&lt;/sub&gt;Sn]]
 |18.3
 |30
 |II
 |ஆம்
 |&lt;ref&gt;{{Cite journal | doi = 10.1103/PhysRev.95.1435| title = Superconductivity of Nb&lt;sub&gt;3&lt;/sub&gt;Sn| journal = Physical Review| volume = 95| issue = 6| pages = 1435| year = 1954| last1 = Matthias | first1 = B. T.| last2 = Geballe | first2 = T. H.| last3 = Geller | first3 = S.| last4 = Corenzwit | first4 = E.| bibcode = 1954PhRv...95.1435M}}&lt;/ref&gt;
 |-
 |[[Niobium-titanium|NbTi]]
 |10
 |15
 |II
 |ஆம்
 |&lt;ref name=m/&gt;
 |-
 |[[Covalent superconductors#Silicon carbide|SiC:B]]
 |1.4
 |0.008
 |I
 |ஆம்
 |&lt;ref name=muranaka&gt;{{Cite journal | doi = 10.1088/1468-6996/9/4/044204| pmid = 27878021| title = Superconductivity in carrier-doped silicon carbide| journal = Science and Technology of Advanced Materials| volume = 9| issue = 4| pages = 044204| year = 2008| last1 = Muranaka | first1 = T. | last2 = Kikuchi | first2 = Y. | last3 = Yoshizawa | first3 = T. | last4 = Shirakawa | first4 = N. | last5 = Akimitsu | first5 = J. | bibcode = 2008STAdM...9d4204M|pmc=5099635}} {{Open access}}&lt;/ref&gt;
 |-
 |[[Covalent superconductors#Silicon carbide|SiC:Al]]
 |1.5
 |0.04
 |II
 |ஆம்
 |&lt;ref name=&quot;muranaka&quot;/&gt;
 |-
 |[[Titanium nitride|TiN]]
 |5.6
 |
 |
 |ஆம்
 |&lt;ref name=prop&gt;{{cite book|page=193|url=https://books.google.com/books?id=pbt-RWodmVAC&amp;pg=PA193|title=Handbook of refractory carbides and nitrides: properties, characteristics, processing, and applications|author =Pierson, Hugh O. | publisher = William Andrew | year =1996| isbn= 0-8155-1392-5}}&lt;/ref&gt;
 |-
 |[[Yttrium borides|YB&lt;sub&gt;6&lt;/sub&gt;]]
 |8.4
 |
 |II
 |ஆம்
 |&lt;ref name=fisk&gt;{{Cite journal | doi = 10.1016/0025-5408(76)90179-3| title = Growth of YB&lt;sub&gt;6&lt;/sub&gt; single crystals| journal = Materials Research Bulletin| volume = 11| issue = 8| pages = 1019| year = 1976| last1 = Fisk | first1 = Z.| last2 = Schmidt | first2 = P. H. | last3 = Longinotti | first3 = L. D. }}&lt;/ref&gt;&lt;ref&gt;{{Cite journal | doi = 10.1016/j.physc.2007.04.135|url=http://www.researchgate.net/publication/243241952_Superconducting_energy_gap_of_YB_6_studied_by_point-contact_spectroscopy| title = Superconducting energy gap of YB&lt;sub&gt;6&lt;/sub&gt; studied by point-contact spectroscopy| journal = Physica C: Superconductivity| volume = 460–462| pages = 626| year = 2007| last1 = Szabó | first1 = P. | last2 = Kačmarčík | first2 = J. | last3 = Samuely | first3 = P. | last4 = Girovský | first4 = J. N. | last5 = Gabáni | first5 = S. | last6 = Flachbart | first6 = K. | last7 = Mori | first7 = T. |bibcode=2007PhyC..460..626S}}&lt;/ref&gt;&lt;ref name =zrb/&gt;
 |-
 |[[Zirconium nitride|ZrN]]
 |10
 |
 |
 |ஆம்
 |&lt;ref name=nitrides&gt;{{Cite journal | doi = 10.1002/sia.740150606| title = Characterization of nitrogen distribution profiles in fcc transition metal nitrides by means of ''Tc'' measurements| journal = Surface and Interface Analysis| volume = 15| issue = 6| pages = 377| year = 1990| last1 = Lengauer | first1 = W. }}&lt;/ref&gt;
 |-
 |ZrB&lt;sub&gt;12&lt;/sub&gt;
 |6.0
 |
 |I
 |ஆம்
 |&lt;ref name=zrb&gt;{{Cite journal | doi = 10.1103/PhysRevB.78.024522| title = Linear and nonlinear low-frequency electrodynamics of surface superconducting states in an yttrium hexaboride single crystal| journal = Physical Review B| volume = 78| issue = 2| pages = 024522| year = 2008| last1 = Tsindlekht | first1 = M. I.| last2 = Genkin | first2 = V. M.| last3 = Leviev | first3 = G. I.| last4 = Felner | first4 = I.| last5 = Yuli | first5 = O.| last6 = Asulin | first6 = I.| last7 = Millo | first7 = O.| last8 = Belogolovskii | first8 = M. A.| last9 = Shitsevalova | first9 = N. Y. 
 | bibcode = 2008PhRvB..78b4522T}}&lt;/ref&gt;
 |}
 == மேற்கோள்கள் ==
 {{Reflist}}
 
 [[பகுப்பு:துப்புரவு முடிந்த தர்மபுரி மாவட்ட ஆசிரியர்கள் தொடங்கிய கட்டுரைகள்]]